Homochiral lanthanoid(iii) mesoxalate metal‒organic frameworks: synthesis, crystal growth, chirality, magnetic and luminescent properties
Gil-Hernández, Beatriz; Maclaren, Jana K.; Höppe, Henning A.; Pasán, Jorge; Sanchiz, Joaquín; Janiak, Christoph; CrystEngComm 14 (2012) 2635–; doi:10.1039/c2ce06496k

data_7207592
_publ_section_title
;
 Homochiral lanthanoid(iii) mesoxalate metal--organic frameworks:
 synthesis, crystal growth, chirality, magnetic and luminescent properties
;
_journal_issue                   8
_journal_name_full               CrystEngComm
_journal_page_first              2635
_journal_paper_doi               10.1039/c2ce06496k
_journal_volume                  14
_journal_year                    2012
_chemical_formula_moiety         'C9 H18 O24 Yb2'
_chemical_formula_sum            'C9 H18 O24 Yb2'
_chemical_formula_weight         856.31
_chemical_name_systematic
;
catena-\D-[triaqua-1.5(\m-dihydroxymalonato-
\kO,O'':O''',O'''')ytterbium(III)]
;
_space_group_IT_number           155
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  'R 3 2"'
_symmetry_space_group_name_H-M   'R 3 2 :H'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   9.55480(10)
_cell_length_b                   9.55480(10)
_cell_length_c                   20.4006(4)
_cell_measurement_reflns_used    9863
_cell_measurement_temperature    203(2)
_cell_measurement_theta_max      35.99
_cell_measurement_theta_min      3.17
_cell_volume                     1612.93(4)
_computing_cell_refinement       'SAINT (Bruker, 2006)'
_computing_data_collection       'APEX2 (Bruker, 2006)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'DIAMOND (Crystal Impact, 2009)'
_computing_publication_material  'publCIF (Westrip, 2009)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      203(2)
_diffrn_measured_fraction_theta_full 0.979
_diffrn_measured_fraction_theta_max 0.979
_diffrn_measurement_device_type  'Bruker APEX2 CCD area detector'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0252
_diffrn_reflns_av_sigmaI/netI    0.0165
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       33
_diffrn_reflns_limit_l_min       -32
_diffrn_reflns_number            21721
_diffrn_reflns_theta_full        36.25
_diffrn_reflns_theta_max         36.25
_diffrn_reflns_theta_min         2.66
_exptl_absorpt_coefficient_mu    8.759
_exptl_absorpt_correction_T_max  0.4458
_exptl_absorpt_correction_T_min  0.1659
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(<i>SADABS</i>; Sheldrick, 1996)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.645
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             1212
_exptl_crystal_size_max          0.32
_exptl_crystal_size_mid          0.19
_exptl_crystal_size_min          0.11
_refine_diff_density_max         1.607
_refine_diff_density_min         -2.094
_refine_diff_density_rms         0.201
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.010(11)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.276
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     63
_refine_ls_number_reflns         1696
_refine_ls_number_restraints     4
_refine_ls_restrained_S_all      1.325
_refine_ls_R_factor_all          0.0137
_refine_ls_R_factor_gt           0.0132
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0183P)^2^+0.6634P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0366
_refine_ls_wR_factor_ref         0.0367
_reflns_number_gt                1662
_reflns_number_total             1696
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c2ce06496k.txt
_cod_data_source_block           ybketo_2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_sg_symbol_Hall     ' R 3 2" '
_cod_original_sg_symbol_H-M      ' R 3 2'
_cod_database_code               7207592